Ag+ colorimetric sensor based on graphene oxide/nano-platinum composite

With the development of society, pollution accidents occur more frequently, and the effects of toxic substances containing silver on human health and environment are increasingly extensive. Therefore, the real-time on-site monitoring of silver ions is urgently needed. Based on the catalase-like properties of graphene/nano-platinum composites and the coupling effect between Pt and Ag+, a simple, unlabeled colorimetric sensing method is proposed to achieve the quantitative detection of Ag+. Under optimal conditions, the detection range of Ag+ by this colorimetric sensing method is 0.5–1000 μM, and the detection limit is 0.5 μM, which is lower than the previously reported detection limit of unlabeled Ag+ colorimetric sensing method, showing higher sensitivity and detection range. Under the same conditions, the sensor has almost no response to interference ions, showing good specific recognition ability. In addition, the colorimetric sensing method can be used to detect Ag+ in actual water samples, serving as a new paradigm for visual detection of Ag+.


Introduction
With the development of industry, environmental problems have become the focus of public concern.Heavy metal ions that cannot be naturally degraded are extremely destructive to nature and human health, and are one of the representative pollutants that cause ecological and environmental problems.Ag + is used in sterilization, purification and deodorization, but if used improperly, it may accumulate in the body and cause argentosis, serious damage to the cell membrane through extracellular mechanisms, skin irritation, stomach pain, organ edema and even death (Khodaparast et al. 2021).Therefore, it is urgent to establish a rapid, sensitive, reliable and low-cost Ag + detection technology.This is of vital significance for food safety, biomedical prevention and environmental protection.
At present, the most commonly used silver ion detection methods include atomic fluorescence spectrometry (Ksa et al. 2019), atomic absorption/emission spectrometry (Yang et al. 2017;Kumar et al. 2019;Karandashev et al. 2019;Winkler. 2020), and inductively coupled plasma mass spectrometry (Shaban et al. 2017).Although these traditional detection methods have high sensitivity and specificity, they have many shortcomings, such as expensive instruments, high operating costs, lack of portability, cumbersome procedures, long time consuming, and strict requirements for operators.In addition, because of the dependence on detection equipment, traditional detection methods are difficult to use in on-site detection, and practicability is poor.Therefore, the development of a rapid, convenient, low-cost, simple and reliable methods that are convenient for on-site detection is the current research hotspot in the field of Ag + detection.
Colorimetric sensing method has the advantages of visual detection results, simple operation, and rapid response.It has been widely concerned and developed rapidly, and can achieve rapid and real-time detection of objects (Zhao et al. 2020;Wu et al. 2019;Yha et al. 2020).Among nanomaterials, graphene and its derivatives have good catalytic performance and have unique layered structure, large specific surface area and active groups on the surface to provide modified active sites for loading other nanomaterials.Consequently, it can be used as a good support material to prepare nanocomposites and has been widely used in the field of colorimetric sensing and detection (Vinotha et al. 2021;Minh et al. 2020;Boruah et al. 2020).Therefore, in this study, graphene oxide has been used as the carrier, and chloroplatinic acid as the precursor to synthesize nanometer catalytic materials with stable structure and high catalytic efficiency, to build a colorimetric sensing detection platform, and to realize the visualization and rapid on-site detection of Ag + .

Chemicals
Silver nitrate (AgNO 3 ), citric acid (C 6 H 8 O 7 ), disodium hydrogen phosphate (Na 2 HPO 4 ), hydrogen peroxide (H 2 O 2 ), chloroplatinic acid (H 2 PtCl 6 ) and 3,3′,5,5′-tetramethylbenzidine (TMB) were purchased from Tianjin Daimao Chemical Reagent Co. Ltd. (China), and graphene oxide was purchased from Shenzhen Qihang Technology Co. Ltd. (China).All metal salt solutions (0.1 M) were prepared from the corresponding metal salts in deionised water.All glassware was cleaned by rinsing several times with tap water and then, re-rinsing with de-high purity water.High purity water obtained using a water purifier (WP-UPT-20, China) was used for reagents preparation.0.1 N Hydrochloric acid and 0.1 N sodium hydroxide, both analytical grade and obtained from Tianjin Damao Chemical Reagent Co. Ltd. (China), were used to adjust the pH.

Synthesis of GO/PtNPs
1.25 mL of graphene oxide (0.5 mg/L) and 0.3 mL of H 2 PtCl 6 solution (10 mM) were mixed homogeneously with 10 mL of ultrapure water.Then, the pH of the system was adjusted to 9.5 with sodium hydroxide (0.1 mol/L) before added with ultrapure water to 12.5 mL.The mixture was then sonicated for 6 h prior to transferring to a hydrothermal reactor (LC-KH-50, LICHEN, China) at 180 °C for 8 h.From this process, a graphene oxide nanoplatinum composites (GO/PtNPs) were obtained.
5 μL of the synthesized GO/PtNPs, 40 μL of TMB (1 mM), and 4 μL of H 2 O 2 (10 M) were mixed and then, fixed to 2000 μL with citrate buffer solution at pH = 5.The absorbance values were measured using a UV-1750 spectrophotometer (Shimadzu, Japan) at 652 nm after 5 min of reaction.

Characterization of the synthesized GO/PtNPs
UV-Vis spectra were obtained using a UV-1750 spectrophotometer from Shimadzu Co. Ltd. of Japan.Fullwavelength scans of graphene and graphene/platinum nanoparticles were performed at 200 nm and 700 nm, respectively, at room temperature.Fourier Transform Infra-Red (FTIR) spectroscopy was performed with a NicoletiS5 (USA) in the range of 4000-400 cm −1 to observe the changes in the surface groups of GO and GO/PtNPs.LabRAM HR confocal micro-Raman spectrometer (France) was used to analyze the changes in GO surface defects before and after synthesis.The crystal structures of GO and GO/PtNPs were evaluated using a PANalytical X-pert3-ray diffractometer (XRD) (Netherlands).The shape and size analyses of the prepared GO/ PtNPs were identified using a JEOL-JEM2100F (Japan) transmission electron microscope (TEM) at 200 kv.An SM-7500F (Japan) X-ray energy spectrometer (EDS) was used for the elemental studies.

Study of catalytic kinetic parameters of GO/PtNPs
A fixed amount of GO/PtNPs (ideal value from synthesis experiment), H 2 O 2 and TMB was placed in a 5 mL test tube.The concentration of H 2 O 2 and TMB was varied at 0.005-0.04M and 0.01-1.5 mM, respectively.Then, citrate buffer solution with pH varied between 2.2 and 8, was added to 2000 μL.The absorbance values were measured using a UV-1750 spectrophotometer (Shimadzu, Japan) at 652 nm.The measurement time was also varied between 1 and 30 min.

Detection ability of the synthesized GO/PtNPs for Ag + ions Specificity and anti-interference analysis
Ag + , Zn 2+ , Cr 6+ , Cu 2+ , Ni 2+ , Al 3+ , Cd 2+ and Ca 2+ solutions were added to 1000 μL citric acid buffer solution with pH 5 and 2 μL GO/PtNPs solution.After well-mixed for 10 min, 4 μL H 2 O 2 (10 M) and 40 μL TMB (1 mM) were added to the system and fixed to 2000 μL with a citric acid buffer solution at pH 5. The absorbance values were measured using a UV-1750 spectrophotometer (Shimadzu, Japan) at 652 nm after reaction for 5 min.

Sensitivity analysis
2 μL GO/PtNPs was mixed with Ag + solution of 0.5-1000 μM and citric acid buffer solution of 1000 μL and pH = 5 until homogeneous for 10 min.Then, 4 μL H 2 O 2 (10 M) and 40 μL TMB (1 mM) were added to 2000 μL in citric acid buffer solution with pH 5.After reaction for 5 min, absorbance values were measured at 652 nm, and standard curves were drawn.

Spike-and-recovery experiment
The practicability of the proposed method was studied by adding different concentrations of Ag + to various environmental water samples (i.e., tap water, pond water and river water).Tap water samples were collected from the municipal pipe network in Jinan, Shandong Province, China; pond water was collected from Jinan, Shandong Province, China; and river water samples were collected from Xiuyuan River in Jinan, Shandong Province, China.
The collected water samples were filtered through a filter membrane with a pore size of 0.22 µm, and Ag + (1, 10, 100, 500 μM) standard solutions were added to the actual water samples.The proposed colorimetric sensing method based on graphene/nano-platinum was used for determination, the experimental results were recorded, and the recovery rate was calculated.

GO/PtNPs characterization TEM characterization analysis
Graphene oxide thin/nano-platinum composites were synthesized by one-step hydrothermal reaction in a solution.In this process, the chloroplatinic acid precursor is directly reduced to Pt NPs, which is anchored on the graphene surface mainly through defects and oxygen functional groups (Satar et al. 2019;Zhao et al. 2021).It is worth noting that due to the residual oxygen-containing groups on the graphene surface, the obtained hybrid can form a well-dispersed aqueous colloid with good stability (Shuang et al. 2017), which is conducive to its application in colorimetric sensing detection.Figure 1 (A) and (B) shows that platinum clusters were fixed on the surface of graphene oxide.The Pt NPs are nearly spherical, distributed between graphene oxide sheets, with particle sizes ranging from 2 to 3 nm.Figure 1C shows the lattice stripes of Pt NPs, whose average crystal plane spacing is 0.2 nm, that is 2.0 Å, corresponding to the {200} and {111} sides of the platinum face-centered cubes.

Raman characterization analysis
Raman spectrum analysis also confirmed the formation of Pt NPs on the graphene sheets (Fig. 2).It can be seen from Fig. 2 that graphene oxide has two characteristic peaks in the range of 1200-1800 cm −1 , namely the D peak at 1369 cm −1 and the G peak at 1614 cm −1 .The D peak represents the disorder-induced feature of carbon materials as the ordered structure of graphene is destroyed after oxidation (Tamalampud et al. 2019).The G peak corresponds to the E 2g phonon vibration in the center of the Brillouin region and is an intrinsic Raman mode of a graphene (Artur et al. 2019;Muniyalakshmi et al. 2020).Partial chemical reduction in GO can bring about structural changes, as evidenced by the shift of the D and G bands to lower wavenumbers and the enhancement of the Raman spectral intensity ratio (I D /I G ) of the D and G bands (Shu et al. 2015).This may be due to the partial reduction in GO, where a large number of sp 3hybridized carbon atoms will be partially deoxygenated to re-form new sp 2 hybridized regions.The re-formed sp 2 regions are smaller than those of GO, so that the average size of the sp 2 regions of the reduced graphene becomes smaller with increased number of sp 2 regions.This is reflected in the Raman spectra as an increase in the value of I D /I G .The Raman spectra of the PtNPs-GO shows that the characteristic peaks of the D and G bands are at 1336 cm −1 and 1593 cm −1 , respectively, and the intensity ratio (I D /I G ) is enhanced (Shu et al., 2015).The peaks can also be seen slightly red-shifted compared with that of pristine GO, and the I D /I G ratio increases from 0.89 to

FT-IR characterization analysis
As shown in Fig. 3, graphene oxide mainly has characteristic peaks at 1053 cm −1 , 1227 cm −1 , 1616 cm −1 , and 1732 cm −1 .The C-O-C telescoping vibration peak at 1053 cm −1 may exist, the face-bending vibration of CH may exist at 1227 cm −1 , and the peaks at 1616 cm −1 and 1732 cm −1 may have C=O stretching vibration.The disappearance of the characteristic peak of C=O stretching vibration at 1732 cm −1 of GO/PtNPs may be due to the reduction reaction during the synthesis of the composites (Ray et al. 2020).The decrease in the characteristic peak of oxygen-containing functional groups was reported to be due to the partial reduction during the hydrothermal reaction of graphene oxide (Muniyalakshmi et al. 2020).

XRD characterization analysis
For precious metal platinum nanoparticles, XRD is a good means to analyze the crystal structure.The comparison of pristine graphene oxide and GO/PtNPs via XRD in Fig. 4 shows an obvious C (002) peak of graphene oxide at about 10.1°.The enhanced characteristic peak at 23.1° indicates that GO is reduced to a certain extent.Moreover, if GO is completely reduced, there should be a weak and wide peak at 26.6° (Legge et al. 2018;Mitra et al. 2021).However, as shown in Fig. 4, there is no peak at 26.6°, which again indicates that GO is only partially reduced rather than completely reduced.The existence form of GO is an important reason why the composite aqueous solution can maintain good dispersion for a long time.Meanwhile, the three diffraction peaks at 40.2°,47.2°and 67.3° correspond to ( 111), ( 200) and ( 220) of the facecentered cubic lattice of platinum, respectively (Wang et al. 2020;Mitra et al. 2020), which proves that platinum nanoparticles were completely loaded on the surface of graphene oxide.

EDS characterization analysis
EDS analysis of GO/PtNPs in Fig. 5 shows it mainly contains three elements: 1.74% carbon, 97.37% oxygen, and 0.89% platinum, which further indicates that the platinum nanoparticles are immobilized on the surface of the GOs, and the composite material of GO/PtNPs is still rich in oxygen-containing functional groups.

Ultraviolet-visible characterization analysis
The UV-Vis absorption spectra of graphene/platinum nanoparticles and graphene oxide are shown in Fig. 6.Graphene oxide shows a relatively strong characteristic peak at wavelength 231 nm, while graphene oxide/platinum nanoparticles have a strong characteristic peak at  267 nm in addition to 231 nm, which is due to the reduction in graphene oxide.This indicates that the graphene oxide in graphene/platinum nanoparticles composites is partially reduced.

Optimization of GO/PtNPs preparation conditions
The catalytic activity of the prepared GO/PtNPs complex is directly related to several influencing factors.The experiment investigated the effects of pH value, H 2 PtCl 6 concentration, hydrothermal time, and hydrothermal temperature on the peroxidase-like catalytic activity of GO/PtNPs complex during the preparation process.The experimental results are shown in Fig. 7. Figure 7A shows the activity test results of catalysts prepared under different pH values.It can be seen that the catalytic activity of GO/PtNPs increases with the increase in pH value, reaching a maximum when the pH value is 9.5, and decreasing with the increase in pH value starting at pH 9.5.This is due to the fact that the Pt 0 precursor can be directly reduced to Pt nanoparticles and grown on the graphene surface under alkaline conditions due to the presence of defects and oxygen-containing functional groups on the surface of graphene oxide lamellae during the hydrothermal reaction (Yoo et al. 2009).
Figure 7B shows the activity test results of the catalysts prepared under different concentrations of H 2 PtCl 6 .It can be seen that the catalytic activity of GO/PtNPs increases with the increase in H 2 PtCl 6 concentration and reaches the maximum when the concentration of H 2 PtCl 6 is 0.24 mM.However, the catalytic activity decreases with the increase in H 2 PtCl 6 concentration greater than 0.24 mM.This is due to the reduction in Pt 4+ to Pt 0 during the hydrothermal reduction process and in situ growth into platinum nanoclusters (refer TEM images in Figure S1).However, too large a concentration of H 2 PtCl 6 can lead to a too large of a particle size of the generated Pt nanoparticles, which reduces the catalyst reactivity (Yuhan et al. 2019).
As shown in Fig. 7C, the catalytic performance of GO/ PtNPs increases from 6 to 9 h and then, decreases with the increase in the reaction time.This shows that the best catalytic performance of GO/ PtNPs was achieved at 9 h of hydrothermal reaction.This is because when the hydrothermal time is too short, Pt 4+ is not sufficiently reduced to Pt 0 , and the remaining Pt 4+ is dispersed in the system and not immobilized on the GO surface (Yoo et al. 2009).When the hydrothermal time is too long, the size of the Pt nanoparticles gradually increases.It was reported that larger size of a nanomaterial reduces the specific surface area and the surface energy generated (Yuhan et al. 2019); thus, the catalytic activity of the composites decreases.
As shown in Fig. 7D, the catalytic activity of GO/PtNPs showed an increasing and then, decreasing trend at a turning point of 180 °C.This is therefore the optimum hydrothermal synthesis temperature.When the temperature of the hydrothermal reaction is lower, Pt 4+ has not yet been reduced to Pt 0 .At higher temperatures, the Pt 0 loaded on the surface of graphene oxide increases continuously.Consequently, the spacing between the graphene oxide lamellae is increased, which effectively reduces the possibility of the agglomeration of graphene oxide.This contributes to the increase in the catalytic activity of the material (Yuhan et al. 2019).
Therefore, through the optimization of experimental conditions in the preparation process of GO/PtNPs, the ideal pH value is 9.5, the concentration of H 2 PtCl 6 is 0.24 mM, the hydrothermal time is 9 h, and the reaction temperature is 180 °C.

Analysis of catalytic kinetics
The synthesized GO/PtNPs have catalase-like properties.With H 2 O 2 and TMB as substrates, the catalytic activity of GO/PtNPs was investigated under the optimal conditions by using the theory and method of enzyme kinetics.In a certain range of substrate concentration, the reaction is typical Michaelis-Menten kinetics as can be seen where ν is the initial rate, V max is the maximum reaction rate, [S] is the substrate concentration, and K m is the Michaelis constant (Shi et al. 2011).K m and V max were obtained from Lineweaver-Burk diagram (Table 1).The K m value of GO/PtNPs under H 2 O 2 conditions is higher than that of enzymes such as GBR (Ray et al. 2017) (see Table 1), which indicates that the activity of GO/PtNPs under H 2 O 2 conditions is higher.In addition, the relatively small K m value is obtained by changing the concentration of TMB.This indicates that TMB has stronger affinity with GO/PtNPs.

Composite material concentration
It can be seen from Fig. 9 that with the increase in the concentration of graphene oxide thin/nano-platinum composite, the trend gradually increases at first and then, reaches plateau at 1.5 absorbance.This is because the higher the concentration of GO/PtNPs, the more catalase-like catalytic sites in the reaction system.So, it can catalyze more effectively the decomposition of hydrogen peroxide to produce hydroxyl radicals to oxidize TMB into oxTMB, and the more obvious the color change (Liu et al. 2012); that is, the greater the absorbance.However, with the increase in GO/PtNPs dosage, the cost will also increase.Therefore, according to the color development ( 1) as shown in Figure S2, when the concentration of composite material is 0.05 μg mL −1 , the material cost can be controlled, and the higher absorbance value can reduce the background interference in the detection process.Therefore, the concentration of GO/PtNPs selected for the experiment is 0.05 μg mL −1 as the detection condition for Ag + .

Reaction time
It can be seen from Fig. 10 that the absorbance is proportional to the reaction time.The absorbance reaches plateau after 20 min.The longer the reaction time, the more sufficient GO/PtNPs can catalyze H 2 O 2 , and the more hydroxyl radicals generated from decomposition will oxidize TMB into oxTMB (Liu et al. 2012), so the absorbance is also larger.However, the longer the reaction time, the higher the time cost of detecting Ag + .Therefore, according to  , the color development was very obvious at 5 min, so 5 min was selected as the optimum time.

pH
It can be seen from Fig. 11 and Figure S4 that the absorbance increases from pH 2 to pH 5 where the absorbance reaches the maximum value of 0.676.The reason is that GO/PtNPs, as a catalase-like material, is greatly affected by pH as other enzymes.When pH is between 4 and 5, this kind of catalase has the highest catalytic activity (Li et al. 2021;Liu et al. 2012).More hydroxyl radicals are decomposed within this pH, causing stronger oxidation ability to TMB, and thus, increases the absorbance.This is consistent with the results of TMB color conditions reported in the literature (Liu et al. 2012).Therefore, the reaction system with pH 5 was selected as the detection condition of Ag + .

Hydrogen peroxide concentration
As shown in Fig. 12, the absorbance values of the system showed a tendency to increase with the increase in hydrogen peroxide concentration before stabilized beyond 0.035 M.This is mainly due to the increase in H 2 O 2 around the catalytic active sites of GO/ PtNPs with the increase in hydrogen peroxide concentration, which decomposes to produce more -OH, and thus, accelerates the color development of TMB (Li et al. 2021;Liu et al. 2012).However, according to the color development shown in Figure S5, the detection can be satisfied when the H 2 O 2 concentration is 0.02 M.

TMB concentration
As shown in Fig. 13, the absorbance value keeps on increasing with the increase in TMB concentration.However, at the TMB concentration of 0.02 mM, the absorbance value is 0.485, which can achieve the detection requirements (refer Figure S6).At the same time, this concentration avoids the phenomenon of a high background value caused by the system's too dark in color.Therefore, the TMB concentration in the subsequent experiments was chosen to be 0.02 mM., and Ca 2+ are selected as interference ions to investigate the specificity of the colorimetric sensing platform.As shown in Fig. 14, the absorbance of the reaction system with interference ions is close to that of the blank group, and there is no obvious inhibition on the properties of GO/PtNPs catalase.However, the absorbance of the reaction system with Ag + decreased significantly, indicating that Ag + significantly inhibited the catalytic ability of GO/PtNPs.This is due to the nonspecific adsorption of Ag + on the surface of GO/PtNPs, which makes the active site on the composite not fully exposed, thus inhibiting the peroxidase-like activity of the composite (Liu et al. 2019).This nonspecific adsorption is that when Ag + is added to the solution, it can coordinate with Pt on GO/ PtNPs.Due to the strong coupling effect between Pt and Ag + , the composite surface is more conducive to the adsorption and accumulation of Ag + , thus reducing the active sites of nano-platinum catalyzing H 2 O 2 on the composite (Chang et al. 2016).Therefore, when Ag + appears in the reaction system, it will inhibit the catalysis of GO/PtNPs on H 2 O 2 , resulting in a significant reduction in the absorbance of the reaction system.

Actual water sample detection
As shown in Fig. 15A, with the measured concentration of Ag + increasing, the color change of the reaction solution gradually weakens.Figure 15B shows the absorbance change curve of the GO/PtNPs-based colorimetric sensing method under different Ag + concentration conditions at the wavelength of 652 nm (the characteristic absorption wavelength of oxTMB).It can be seen from the figure that the change of solution absorbance weakens with the increase in Ag + concentration.This is because Ag + will absorb nonspecific on the surface of the composite material, so that the active sites on the composite material cannot be completely exposed, thus inhibiting the peroxidase-like activity of the composite material (Chang et al. 2016).Figure 15C shows the concentration of Ag + (0.5-1000 μM) and the absorbance of the solution when the system reacts for 5 min.It can be seen that when the concentration of Ag + is 0.5-1000 μM, it shows a good exponential relationship with the absorbance of the system, and the linear fitting equation from Fig. 15D is shown in Eq. 2; This provides a basis for the quantitative analysis of Ag + .The limit of quantification (LOQ) of this sensing method is 0.5 μM, which is the lowest concentration of the sample that can be detected in the experiment.
In order to explore its reproducibility, Ag + concentration is configured as 0.5, 1, and 10 μM.The relative standard deviations (RSDs, n−3) of the obtained results are 5.58%, 1.95% and 6.16%, respectively, which proves that the sensing method has good reproducibility.In addition, Ag + samples with different concentrations were prepared and the accuracy of the sensing method was investigated by spiking recovery experiment.Based on the obtained linear fitting equation, the sample Ag + concentration is calculated from the solution absorbance.The calculation results are shown in Table 2.It can be seen that the recovery rate of the method is 96.46-104.57%,within an acceptable range, indicating that the accuracy and precision of this sensing method are good and can be used for the quantitative detection of Ag + in actual water samples.
As shown in Table 3, the detection range of silver ion based on this colorimetric platform is 0.5-1000 μM.Compared with sensors of the same kind, the detection range is wider and the application conditions are wider.Moreover, the detection limit is 0.5 μM, which is more sensitive compared with the same kind of colorimetric sensor.

Detection mechanism of Ag + ion
The principle of the colorimetric sensor is based on the redox reaction between the nano-catalytic material and the substance to be tested to generate a chemical signal, which is outputted as an optical signal through the color change of the color-developing substrate, thus realizing the detection process of the target (Chen et al .The synthesized GO/PtNPs have superior peroxidase-like properties that can catalyze the decomposition of hydrogen peroxide.The hydroxyl radical generated from the decomposition can oxidize the hydrogen peroxide substrate 3,3′,5,5′-tetramethylbenzidine (TMB), which can be changed from a colorless substance to a blue product.When the system contains Ag + , it mainly reacts with Pt 0 on the surface of graphene oxide in a redox reaction to produce silver-platinum bimetallic nanoparticles (Ag@PtNPs), resulting in poor affinity with the substrate TMB.This inhibits the catalytic activity of the composite material, leading to a lighter color and lower absorbance of the system.The higher the concentration of Ag + , the lighter the color of the system, and the lower the absorbance value.The qualitative analysis of Ag + can be achieved by the naked eye through the change of color.In addition, according to Lambert's Beer's law, the quantitative relationship between the absorbance value and the concentration of Ag + can be established, and finally, the quantitative concentration of Ag + is achieved.This mechanism of Ag + colorimetric sensor is shown in Fig. 16.

Conclusion
In this paper, GO/PtNPs were synthesized by one-step hydrothermal method, and the visual detection of Ag + was realized by using the catalase-like properties of the material and the nonspecific adsorption of Ag + on the surface of the composite.The main conclusions are as follows: a. GO/PtNPs were prepared by hydrothermal synthesis, and GO/PtNPs were evaluated by TEM, Raman, and XRD characterization.The weak red shift of D band and G band under Raman characterization indicates that graphene oxide was only partially reduced.The characteristic peak of face-centered cubic structure with unique precious metal platinum appeared in the XRD characterization, indicating that nano-platinum was completely loaded on the surface of graphene oxide.The catalytic activity of GO/PtNPs was investigated using H 2 O 2 and TMB as substrates by using the theory and method of enzyme kinetics.b.By optimizing the synthesis conditions of GO/PtNPs, it was found that the composite with good catalytic performance could be obtained by pH 9.5, H 2 PtCl 6 of 0.25 mM, reaction temperature of 180 ℃, and reaction time of 9 h.The reaction conditions for the detection of Ag + were explored through single factor experiments.The composite concentration, reaction time and pH of the system in the reaction process were optimized.The final detection condition selects the concentration of GO/PtNPs as 0.005 μg mL −1 ,   reaction time of 5 min and system pH of 5 were used as the detection conditions for Ag + .c. Compared with the effect of eight metal ions, this method has good selectivity for Ag + .At the same time, Ag + in different concentration gradients and Ag + in actual water samples of tap water, pond water and river water are detected.The results show that the detection range of this method is 0.5-1000 μM and the detection limit is 0.5 μM.The spike-andrecovery rates of tap water, pond water and river water range from 96.61 to 104.57%, and the detection time is 5 min.Compared with sensors of the same kind, the detection range is wider, more sensitive, and the application conditions are wider, thus offering a broader application prospect.

Fig. 2
Fig. 2 Raman spectra of GO and GO/PtNPs

Fig. 6
Fig. 6 Ultraviolet-visible spectral characterization of GO and GO/ PtNPs

Fig. 15 A
Fig. 15 A Photographs of color change of solution of detection system at different concentrations of Ag + ; B Colorimetric sensing method based on GO/PtNPs absorbance versus time curve of different concentrations of Ag + ; C The relationship between the absorbance and the concentration of Ag + ; and D Linear fitting curve between absorbance value and-log [Ag + ].Reaction condition: GO/PtNPs 0.047 μg/mL, H 2 O 2 0.02 M, TMB 0.02 Mm, pH = 5, t = 5 min, λ = 652 nm

Fig. 16
Fig. 16 Detection mechanism of Ag + ion colorimetric sensor based on GO/PtNPs

Table 1
Comparison of apparent Michaelis constant (K m ) and maximum reaction rate (V max ) between GO/PtNPs and other catalases

Table 2
Detection of Ag + in actual water samples

Table 3
Performance comparison of several silver ion sensors